Multiple exciton generation in chiral carbon nanotubes: Density functional theory based computation Andrei Kryjevski, Deyan Mihaylov, Svetlana Kilina, and Dmitri Kilin Citation: The Journal of Chemical Physics 147, 154106 (2017); View online: https://doi.org/10.1063/1.4997048 View Table of Contents: http://aip.scitation.org/toc/jcp/147/15 Published by the American Institute of Physics Articles you may be interested in Cluster decomposition of full configuration interaction wave functions: A tool for chemical interpretation of systems with strong correlation The Journal of Chemical Physics 147, 154105 (2017); 10.1063/1.4996044 Electronic energy transfer through non-adiabatic vibrational-electronic resonance. I. Theory for a dimer The Journal of Chemical Physics 147, 154308 (2017); 10.1063/1.5005835 Communication: Master equations for electron transport: The limits of the Markovian limit The Journal of Chemical Physics 147, 151101 (2017); 10.1063/1.5000747 One-particle many-body Green’s function theory: Algebraic recursive definitions, linked-diagram theorem, irreducible-diagram theorem, and general-order algorithms The Journal of Chemical Physics 147, 044108 (2017); 10.1063/1.4994837 Resonant-convergent second-order nonlinear response functions at the levels of Hartree–Fock and Kohn– Sham density functional theory The Journal of Chemical Physics 147, 144109 (2017); 10.1063/1.4991616 Spectroscopic properties of photosystem II reaction center revisited The Journal of Chemical Physics 147, 115102 (2017); 10.1063/1.4997527 THE JOURNAL OF CHEMICAL PHYSICS 147, 154106 (2017) Multiple exciton generation in chiral carbon nanotubes: Density functional theory based computation Andrei Kryjevski,1 Deyan Mihaylov,1 Svetlana Kilina,2 and Dmitri Kilin2 1 Department 2 Department of Physics, North Dakota State University, Fargo, North Dakota 58108, USA of Chemistry, North Dakota State University, Fargo, North Dakota 58108, USA (Received 20 July 2017; accepted 26 September 2017; published online 20 October 2017) We use a Boltzmann transport equation (BE) to study time evolution of a photo-excited state in a nanoparticle including phonon-mediated exciton relaxation and the multiple exciton generation (MEG) processes, such as exciton-to-biexciton multiplication and biexciton-to-exciton recombination. BE collision integrals are computed using Kadanoff-Baym-Keldysh many-body perturbation theory based on density functional theory simulations, including exciton effects. We compute internal quantum efficiency (QE), which is the number of excitons generated from an absorbed photon in the course of the relaxation. We apply this approach to chiral single-wall carbon nanotubes (SWCNTs), such as (6,2) and (6,5). We predict efficient MEG in the (6,2) and (6,5) SWCNTs within the solar spectrum range starting at the 2E g energy threshold and with QE reaching ∼1.6 at about 3E g , where E g is the electronic gap. Published by AIP Publishing. https://doi.org/10.1063/1.4997048 I. INTRODUCTION Efficiency of photon-to-electron energy conversion in nanomaterials is an important issue that has been actively investigated in recent years. For instance, it is envisioned that efficiency of the nanomaterial-based solar cells can be increased due to carrier multiplication, or multiple exciton generation (MEG) process, where absorption of a single energetic photon results in the generation of several excitons.1–3 In the course of MEG, the excess photon energy is diverted into creating additional charge carriers instead of generating atomic vibrations.3 In fact, phonon-mediated electron relaxation is a major time-evolution channel competing with the MEG. The conclusion about MEG efficiency in a nanoparticle can only be made by simultaneously including MEG, phononmediated carrier relaxation, and, potentially, other processes, such as charge and energy transfer.4,5 In the bulk semiconductor materials, MEG in the solar photon energy range is known to be inefficient.6–8 In contrast, in nanomaterials, MEG is expected to be enhanced by spatial confinement, which increases electrostatic electron interactions.3,9–11 Internal quantum efficiency (QE) is the average number of excitons generated from an absorbed photon. It is a potent measure of MEG efficiency. QE exceeding 100% has been measured in recent experiments on, e.g., silicon and germanium nanocrystals, and in nanoparticle-based solar cells.12–17 Also, MEG has been observed in single-wall carbon nanotubes (SWCNTs) using transient absorption spectroscopy13 and the photocurrent spectroscopy;18 QE = 1.3 at the photon opt opt energy ~ω = 3Eg , where Eg is the optical gap, was found in the (6,5) SWCNT. Theoretically, MEG in SWCNTs has been investigated using tight-binding approximation with QE up to 1.5 predicted in the (17,0) zigzag SWCNT.19,20 It is understood that in semiconductor nanostructures MEG is dominated by the impact ionization process.21,22 Therefore, MEG 0021-9606/2017/147(15)/154106/9/$30.00 QE requires calculations of the exciton-to-biexciton decay rate (R1→2 ) and of the biexciton-to-exciton recombination rate (R2→1 ), the direct Auger process, and, of course, inclusion of carrier phonon-mediated relaxation. In quasi one-dimensional systems, such as SWCNTs, accurate description of these processes requires inclusion of the electron-hole bound state effects—excitons.23 Recently, Density Functional Theory (DFT) combined with the many-body perturbation theory (MBPT) techniques has been used to calculate R1→2 and R2→1 rates, and the photon-to-bi-exciton, R2 , and photon-to-exciton, R1 , rates in two chiral (6,2) and (10,5) SWCNTs which have different diameters, including exciton effects.24 QE was then estimated as QE = (R1 + 2R2 )/(R1 + R2 ). However, phonon relaxation was not included. Also, R1→2 and R2→1 for the singlet fission (SF) channel of MEG for these systems have been computed in Ref. 25. The results suggested that efficient MEG in chiral SWCNTs, both in all-singlet and SF channels, might be present within the solar spectrum range with R1→2 ∼ 1014 s1 , while R2→1 /R1→2 ≤ 10−2 , it was estimated that QE ' 1.2−1.6. However, MEG strength in these SWCNTs was found to vary strongly with the excitation energy due to highly non-uniform density of states. In contrast, the MEG rate calculation done for (6,2) with Cl atoms adsorbed to the surface indicated that MEG efficiency in these systems could be enhanced by altering the low-energy electronic spectrum via, e.g., surface functionalization.25 Carrier multiplication and recombination without exciton effects and phonon-mediated relaxation were studied using coupled rate equations in coupled silicon nanocrystals in Ref. 26. In this work, we develop and apply a Boltzmann transport equation (BE) approach to study MEG in chiral SWCNTs including both exciton multiplication and recombination, i.e., the Auger processes, and the phononmediated exciton relaxation. The Kadanoff-Baym-Keldysh, or 147, 154106-1 Published by AIP Publishing. 154106-2 Kryjevski et al. J. Chem. Phys. 147, 154106 (2017) non-equilibrium Green’s function (NEGF), formalism—a generalization of DFT-based MBPT for a non-equilibrium state—allows one to use perturbation theory to calculate collision integrals in the transport equation for time evolution of a weakly non-equilibrium photoexcited state.27–29 Notably, while BE coefficients can be computed to a given order in MBPT, the BE itself is non-perturbative. We calculate QE for the (6,2) and (6,5) SWCNTs. This work aims to provide insights into dynamics of photoexcited SWCNTs and its dependence on the chirality, diameter, and excitation energy. The paper is organized as follows. Section II contains the description of the methods and approximations used in this work. Section III contains the description of the atomistic models used in this work and of the simulation details. Section IV contains discussion of the results obtained. Conclusions and outlook are presented in Sec. V. II. THEORETICAL METHODS AND APPROXIMATIONS A. Electron Hamiltonian in the KS basis and approximations The electron field operator ψα (x) and the annihilation operator of the ith Kohn-Sham (KS) state aiα are related via X ψα (x) = φiα (x)aiα , (1) i where φiα (x) is the ith KS orbital and α is the electron spin index.30,31 Here we only consider spin unpolarized states with φi↑ = φi↓ ≡ φi ; also {aiα , ajβ+ } = δij δαβ , { aiα , ajβ } = 0. Then, in terms of aiα , aiα+ , the Hamiltonian of electrons in a CNT is (see, e.g., Refs. 24, 25, and 32) X H= i a†iα aiα + HC − HV + He−exciton , (2) Tamm-Dancoff approximation a spin-zero exciton state can be represented as35,36 X X 1 α † aeσ ahσ |g.s. i , (5) |α i0 = Bα† |g.s. i = √ Ψeh 2 eh σ=↑,↓ where the index ranges are e > HO, h ≤ HO, where HO is the highest occupied KS level, LU = HO + 1 is the lowest unocα are the singlet exciton cupied KS level, and where Bα† , Ψeh creation operator and wavefunction, respectively. Then, the last term in the Hamiltonian (2) is He−exciton X X 1 α † ahσ aeσ (Bα + Bα† ) + h.c. eh − E α Ψeh = √ 2 ehα σ X + E α Bα† Bα , eh = e − h , (6) α Eα where are the singlet exciton energies. The He exciton term can be seen as the result of re-summation of perturbative corrections to the propagating electron-hole state whereby exciton states emerge instead of electron-hole pairs (see, e.g., Refs. 37 and 38); it describes coupling of excitons to electrons and holes, which allows systematic inclusion of excitons in the perturbative calculations.38–41 See Ref. 25 for more details. To determine exciton wave functions and energies, one solves the Bethe-Salpeter equation (BSE).35,36 In the static screening approximation commonly used for semiconductor nanostructures (see, e.g., Refs. 42–44), the BSE is43 X α ( eh − E α ) Ψeh + (KCoul + Kdir )(e, h; e0, h 0)Ψeα0 ,h0 = 0, e0 h0 KCoul = 1 X Vijkl a†iα a†jβ akβ alα , 2 ijkl α,β e2 = dxdy φ∗i (x)φ∗j ( y) φk (y)φl (x). |x − y| HC = Vijkl (3) The HV term prevents double-counting of electron interactions ! X † ∗ HV = aiα dxdy φi (x)VKS (x, y)φj (y) ajα , (4) ij where V KS (x, y) is the KS potential consisting of the Hartree and exchange-correlation terms (see, e.g., Refs. 33 and 34). Photon and electron-photon coupling terms are not directly relevant to this work and, so, are not shown, for brevity. In this work, we will consider singlet excitons only, leaving triplet exciton effects for future work. Before discussing the last term in the Hamiltonian (2), let us recall that in the Vq2 q,0 Kdir = − iα where i↑ = i↓ ≡ i is the ith KS energy eigenvalue. Typically, in a periodic structure i = {n, k}, where n is the band number and k is the lattice wavevector. However, for reasons explained in Sec. III, here KS states are labeled by just integers. The second term is the (microscopic) Coulomb interaction operator X 8πe2 ρeh (q)ρ∗0 0 (q) eh , (7) 2 ∗ 1 X 4πe ρee0 (q)ρhh0 (q) , V q,0 q2 − Π(0, −q, q) where ρji (p) = X φ∗j (k − p)φi (k) (8) k is the transitional density and 8πe2 X Π(ω, k, p) = ρij (k)ρji ( p) V ~ ij ! θ −j θ i θ j θ −i × − , ω − ωij + iγ ω − ωij − iγ X X X X ~ωij = ij , θi = , θ −i = i i>HO i (9) i ≤HO is the random phase approximation (RPA) polarization insertion (see, e.g., Ref. 30). A major screening approximation used in this work [see Eqs. (7) and (22)] is that Π(0, k, p) ' Π(0, −k, k)δk,−p corresponding to Π(0, x, x 0) ' Π(0, x − x 0), i.e., to the uniform medium approximation. See Refs. 24 and 25 for more details and discussion of applicability to SWCNTs. Here, we have used hybrid Heyd-Scuseria-Ernzerhof (HSE06) exchange correlation functional in our DFT simulations45,46 as it has been successful in reproducing electronic gaps in various semiconductor nanostructures (e.g., Refs. 34, 154106-3 Kryjevski et al. J. Chem. Phys. 147, 154106 (2017) 47, and 48). (See, however, Ref. 49.) Therefore, using the HSE06 functional is to substitute for GW corrections to the KS energies—the first step in the standard three-step procedure.35,50 So, single-particle energy levels and wave functions are approximated by the KS i and φi (x) from the HSE06 DFT output. While inclusion of GW corrections would improve accuracy of our calculations, it is unlikely to alter our results and conclusions qualitatively. Next, we describe how the BE follows from the Keldysh MBPT which is the approach to the description of time evolution of a photoexcited state used in this work. B. Boltzmann transport equation from Kadanoff-Baym-Keldysh formalism Description of time evolution of a photoexcited nanoparticle should be comprehensive and, thus, include dynamics of electrons, phonons, and, also, photons if one aims to include absorption and recombination. For instance, to study MEG one needs to allow carrier multiplication to “compete” with the phonon-mediated relaxation, and, possibly, other processes, such as the energy and charge transfer. The Boltzmann transport equation (BE) is a suitable approach to this problem. The Kadanoff-Baym-Keldysh formalism—a generalization of MBPT for non-equilibrium states—allows one to calculate collision integrals in the transport equation for time evolution of a weakly non-equilibrium photoexcited state.27–29 As noted above, while BE collision integrals can be computed to a given order in MBPT, the BE itself provides non-perturbative description. Typically, a simple relaxation time approximation is used for the collision integral.29 See, e.g., Ref. 51 for a recent application. However, it is known that the equation of motion for the Keldysh propagator G + in the quasi-classical limit reduces to the transport equation.29 This allows for systematic calculations of the collision integrals using Keldysh MBPT. Let us consider correlation function G−+ α (t1 , t2 ) † = hN | Bα (t2 )Bα (t1 )|N i , where |N i is some weakly nonequilibrium state, such as a photoexcited state at finite temperature, and Bα (t) is the αth exciton state Heisenberg operator. Note that G−+ α is related to the density matrix. The equation of motion for G−+ α (t1 , t2 ) is ! Eα d − G−+ (t , t ) = dt3 Σα−− (t1 , t3 )G−+ i α (t3 , t2 ) α 1 2 dt1 ~ (10) + Σα−+ (t1 , t3 )G++ α (t3 , t2 ) , where Σα−+ , Σα−− , G++ α are the Keldysh self-energies and correlators, respectively. The BE is obtained when the slow t = (t 1 + t 2 )/2 and fast (intrinsic) t 0 = t 1 t 2 times are introduced (see paragraph 95 of Ref. 29 for details). It describes slow timeevolution of a weakly non-equilibrium state. For instance, the t1 → t2 components of G−+ α are the exciton occupation numbers: nα (t) = G−+ (t, t). It is the set of nα (t) that describes the α non-equilibrium state |N i . Then the BE for the (slow) time evolution of a photo-excited state is ṅα = iΣα−+ (n; ωα ) (1 + nα ) − iΣα+− (n; ωα ) nα , ωα = Eα , ~ (11) where Σα−+ , Σα+− are the leading Keldysh exciton self-energies, which depend on the slowly varying occupation numbers. Different contributions to the self-energies that correspond to different processes will be discussed below. Note that the r.h.s. of Eq. (11) has the expected “gain”–“loss” term structure. The approach is applicable if ṅα (t) ωα , which is the quasi-classicality condition in this case. Solving the system of equations (11) with the initial condition nα (t = 0) , 0 for ~ωα = ~ω, where the excitation energy ~ω corresponds to, e.g., an absorption peak, will yield description of relaxation in a photo-excited nanoparticle. As mentioned above, here we aim to describe dynamics of a photoexcited SWCNT including electron-hole bound state (exciton) effects and taking into account (I) phonon-mediated relaxation, i.e., the non-adiabatic processes and (II) excitonto-bi-exciton decay and bi-exciton recombination, i.e., inverse and direct Auger processes. Collision integrals for these two processes will be described in Subsections II C and II D. Then, in order to calculate internal QE, one 1. populates exciton with energy E; the initial state is ni (0) = nin δiα , E α = E; 2. solves BE including (a) phonon emission and absorption terms, and (b) exciton-to-bi-exciton decay and recombination; 3. adds up the occupation numbers of excitons generated after the occupancies have plateaued as t → ∞. (Recall that recombination occurring on a much longer time scale is not included here.) After the initial state averaging, P nα (t → ∞) . (12) QE(E) = α nin C. Electron-phonon interaction In order to include phonon terms and the electron-phonon coupling, Hamiltonian (2) is augmented by Nion X PI2 1 X ZI ZJ e2 + VNN , VNN ' , HN = 2MI 2 I,J |RI − RJ | I=1 (13) where PI , RI , M I , Z I are the Ith ion momentum, position, mass, and effective charge number of valence electrons, respectively; PI , RI are the ion momentum and position operators, respectively, I = 1,. . . ,N ion . One sets RI = R0I + rI , where the equilibrium ion positions R0I corresponding to the energy minimum have been found by, e.g., the DFT geometry relaxation procedure and rI are small oscillations about equilibrium. This leads to the following phonon and electron-phonon terms in the Hamiltonian (see, e.g., Refs. 52 and 53): δHe−ph = 3NX ion −6 ν=1 ~ων cν† cν + ! X 1 + gνij a†iσ ajσ ( cν† + cν ), 2 ijνσ (14) where cν is the phonon annihilation operator and the electronphonon couplings are53 s ∗ (p) p · Uν e−ip· RI Ni 2 X X ρ 4πiZ e ~ I ji I gνij = . V 2ων MI p p2 − Π(0, −p, p) I=1 (15) 154106-4 Kryjevski et al. J. Chem. Phys. 147, 154106 (2017) This is similar to the frozen photon approximation.54,55 Our approach is applicable to the systems where atoms undergo small oscillations about their equilibrium positions; the electronic states are approximated using equilibrium atomic positions R0I . Normal frequencies, ων , and mode decompositions, UνI , are calculated using DFT software, such as Vienna ab initio simulation program (VASP). The pseudopotential v(x, RI ) felt by the valence electrons is approximated here by the Coulomb interaction, which is also (approximately) screened.30 The O(rI2 ) contribution to δHe ph (see, e.g., Ref. 56) is neglected since it does not contribute to the exciton-phonon Keldysh couplings at the leading one-phonon level. More generally, the O(rI2 ) term’s contribution is suppressed due to screening of v(x, RI ).30,57 So, in order to describe phonon-mediated relaxation in a nanoparticle, one includes electron-phonon interactions described in Eqs. (14) and (15). The corresponding Feynman diagrams are shown in Fig. 1. In SWCNTs, sub-gaps in the electronic energy spectrum are sizable enough for the twophonon processes [Fig. 1(b)] to be relevant. With the one- and two-phonon processes included, the BE is µν (G2 )αβ cpp chh chp cph ṅα = X αµ + µ (G1 )αβ nβ nµ − nα nβ + nµ + 1 δ ωα − ωβ − ωµ X αµν µν (G2 )αβ ( nµ nν nβ − nα − nα nβ + 1 nµ + nν − nα nβ + 1 ) × δ ωα − ωβ − ωµ − ων − {α ↔ β}, where (16) " nν ' exp # ! −1 ~ων −1 kB T (17) and µ (G1 )αβ 2 β *.X µ α ∗ θ −i θ j θ k gjk Ψji Ψki . ijk , 2 X β + µ α ∗ / + θ i θ −j θ −k gjk Ψij Ψik / , ijk - 2π ' 2 ~ (18) µ where (G1 )αβ are the dominant terms of the effective excitonphonon couplings and T is the temperature. Also, 2 X X 1 cpp + chh + cph + chp , ωα + ωµ − ωσ + iδ pkqjli σ β ∗ σ α ∗ σ ωij − ωσ Ψiq θ θθ Ψlk Ψlp ωlp − ωσ θ i θ −j θ −q Ψij µ ν −k l −p , = gpk gqj ωlp − ωα − ωµ − iδ ωij − ωα − ωµ − iδ σ (ω − ω ) Ψ β ∗ α Ψσ ∗ ω − ω θ θ θ Ψ θ θ θ Ψ q σ −k l lk pi σ −i j p lk pi ji qk µ = gpj gνql , ωα + ωµ − ωpi + iδ ωα + ωµ − ωlk + iδ β α Ψσ ∗ ω − ω σ ω −ω θ θ θ Ψ θ θ θ Ψ Ψiq ∗ p σ k −l pl i −j −q ij σ ij kl pl µ = gνjq gpk , ωα + ωµ − ωpl + iδ ωij − ωα − ωµ − iδ β σ ∗ ω −ω σ θ θ θ Ψα Ψlp ψqi ∗ σ θ −i θ j θ q Ψji ωji − ω σ lp µ ν −k l −p lk = gkp gqj , ωlp − ωα − ωµ − iδ ωα − ωji + ωµ + iδ 2π ' 4 ~ where δ is the small width parameter set here to the temperature scale 25 meV. Both phonon emission and absorption from the thermal bath by either the electron or the hole within the exciton are included in Eq. (16). The twophonon processes where one phonon is emitted and the other one is absorbed are not included in Eq. (16) for (19) technical simplicity. Also, in this perturbative approach, phonon occupation numbers are approximated by their equilibrium values [see Eq. (17)], which is another technical simplification. In the above and in the following expressions, only the terms leading in the ratio of the typical exciton binding energy FIG. 1. Typical Feynman diagrams for the Σ+ describing exciton-phonon coupling. Shown in (a) and (b) are the one- and two-phonon processes, respectively. Thin solid lines stand for the KS state propagators, thick solid lines depict excitons, and dashed lines depict phonons. The + contributions obtain when + and are interchanged. 154106-5 Kryjevski et al. J. Chem. Phys. 147, 154106 (2017) to the gap ( binding /Eg ) < 1 are shown for brevity. But full expressions have been included in the actual calculations. D. MEG terms Transport equations that describe exciton-to-biexciton decay and biexciton-to-exciton recombination are dnγ X γ = Rαβ nα nβ − nγ nα + nβ + 1 αβ dt × δ ωα + ωβ − ωγ , X dnβ dnα γ + nβ =− Rαβ nα nβ − nγ nα + nβ + 1 nα γ dt dt × δ ωα + ωβ − ωγ , (20) γ where Rαβ are −+ +− Σα , Σα shown the rates from the MEG contributions to in Fig. 2. In (20), the first equation describes the impact ionization (I.I.) process where exciton γ decays into excitons α and β and the second equation describes the inverse recombination process (direct Auger). The leading order rate expressions are (α, β, γ subscripts are omitted for brevity)24 γ Rαβ = Rp + Rh + R̃p + R̃h δ(ωγ − ωα − ωβ ), X 2 W θ θ (Ψβ )∗ θ θ θ Ψγ Ψα ∗ , i −j −k ij jlnk l −n ik ln ijkln X 2 2π β γ Rh = 2 2 Wjlnk θ −l θ n Ψnl θ −i θ j θ k (Ψji )∗ Ψkiα . ~ ijkln 2π R =2 2 ~ p (21) The expressions for R̃h and R̃p are the same as the ones for Rh , Rp with W jlnk replaced by W jlkn and divided by 2. In the above, X 4πe2 ρ∗kj (q)ρln ( q) (22) Wjlnk = V q2 − Π(0, −q, q) q,0 is the (approximate) screened Coulomb matrix element. Strictly speaking, here we are working to the second order in the screened Coulomb interaction. This refers to the electron → trion, hole → trion sub-processes in Fig. 2, i.e., the trion is created in the course of a single Coulomb interaction. However, as discussed above, the electron-hole interactions that form the excitons are included to all orders. Also, in this work, a biexciton state is approximated by a pair of non-interacting excitons. III. COMPUTATIONAL DETAILS The optimized SWCNT geometries, KS orbitals, and energy eigenvalues have been obtained using the ab initio total energy and molecular dynamics program VASP (Vienna ab initio simulation program) with the hybrid HeydScuseria-Ernzerhof (HSE06) exchange correlation functional45,46 using the projector augmented-wave (PAW) pseudopotentials.58,59 Applying the conjugated gradient method for atomic position relaxation, the structures were relaxed until residual forces on the ions were no greater than 0.05 eV/Å. The momentum cutoff defined by ~2 k 2 ≤ Emax , (23) 2m where m is the electron mass, was chosen at Emax = 400 eV. The energy cutoffs determined by the number of KS orbitals included in the simulations were chosen so that imax − HO ' LU − imin ≥ 3 eV, where imax , imin are the highest and the lowest KS labels included in simulations. SWCNT atomistic models were placed in the finite volume simulation boxes with periodic boundary conditions. In the axial direction, the box size was chosen to accommodate an integer number of unit cells. In the other two directions, the SWCNTs have been kept separated by about 1 nm of vacuum surface-tosurface which excluded spurious interactions between their periodic images. As discussed in Ref. 24, we have found reasonably small (about 10%) variation in the single particle energies over the Brillouin zone when three unit cells were included in the DFT simulations.24 Therefore, in (6,2) simulations have been done at the Γ point including three unit cells. In our approximation, lattice momenta of the KS states, which are suppressed by the reduced Brillouin zone size, have been neglected. Due to high computational cost, for (6,5) SWCNT only one unit cell was included. However, we checked that this size-reduced model reproduced the absorption spectrum features with the accuracy similar to other SWCNTs.25 As explained before in Ref. 24, the rationale for including multiple unit cells instead of the Brillouin zone sampling in the DFT simulations is that surfaces of these SWCNTs are to be functionalized. Inclusion of several unit cells keeps the concentration of surface dopants reasonably low. The atomistic models of the optimized nanotubes are shown in Fig. 3. In this work, all the DFT simulations have been done in a vacuum which is to approximate properties of these SWCNTs dispersed in a non-polar solvent. FIG. 2. Exciton self-energy Feynman diagrams relevant for the exciton → bi-exciton and bi-exciton → exciton processes. Thin solid lines stand for the KS state propagators, thick solid lines depict excitons, and zigzag lines depict screened Coulomb potential. The diagrams on the left and the right correspond to the exchange and direct channels, respectively. Not shown for brevity are the similar diagrams with all the Fermion arrows reversed and with + and interchanged, 154106-6 Kryjevski et al. FIG. 3. Atomistic models of chiral SWCNTs. Shown in (a) is SWCNT (6,2). Three unit cells have been included in the simulations. In (b) is SWCNT (6,5). Only one unit cell is included due to computational cost restrictions. IV. RESULTS AND DISCUSSION First, we have simulated relaxation of an energetic exciton state corresponding to the absorption peak E 22 including electron-phonon interactions only. The results are shown in Fig. 4. Phonon spectra for CNTs (6,2) and (6,5) computed using VASP are in Fig. 4(a). Shown in Fig. 4(b) are the occupancies of the E 22 peak exciton states in CNT (6,5). As expected, the initial excitation is cascading down in energy. Intermediate states are being excited and subsequently decay in the course of the relaxation. An exponential fit to the predicted nE22 (t) curve has yielded decay constant τ 22 = 16.7 fs. The available experimental results are for (6,5) in the aqueous solution where τ 22 = 120 fs was reported.60 For SWCNTs of unspecified chiralities immersed in polyethylene glycol J. Chem. Phys. 147, 154106 (2017) and in polymethylmethacrylate, τ22 ' 40 fs was reported.61,62 So, while direct comparison is not possible at this time, it is likely that our prediction for τ 22 is underestimated. This is as expected and is in line with other predictions of our approach which tends to overestimate the strength of couplings. Overall, this confirms applicability of our method for semi-quantitative description of photoexcited chiral SWCNT dynamics. Shown in Figs. 4(c) and 4(d) are the few low-energy exciton occupancies resulting from the excitation at the E 22 peak energy for (6,5) and (6,2), respectively. The excitation goes through several transient states before forming a terminal steady state where only few low-energy levels are occupied. In (6,2) the relaxation time from the E 22 excitation is about 100 fs [Fig. 4(d)], while in (6,5) the E 22 relaxation time is predicted to be two orders of magnitude longer [Fig. 4(c)]. The results suggest that relaxation rates in CNTs strongly depend on the diameter and chirality. This is as expected. It is known that opto-electronic properties of SWCNTs depend on chirality.63 In chiral CNTs, charge density distribution forms continuous “threads” along the lines of C–C conjugation. But orientation of these lines depends on the chirality index. So, spatial distribution of electronic density in low-energy states is chirality-dependent. Therefore, all major electronic properties of CNTs, including MEG and phonon-relaxation, are chirality-dependent. FIG. 4. Phonon densities of states (DOSs) for the two CNTs are shown in (a). Shown in (b) are the occupation numbers of the exciton states corresponding to the E 22 peak energy in CNT (6,5). In (c) and (d) are the few low-energy exciton occupancies after excitation at the E 22 peak energy in (6,5) and (6,2), respectively. 154106-7 Kryjevski et al. J. Chem. Phys. 147, 154106 (2017) FIG. 5. Exciton and bi-exciton densities of states (DOSs) for the CNT (6,2) (E g = 0.98 eV) and CNT (6,5) (E g = 1.09 eV) are shown in (a) and (b), respectively. Exciton DOSs are the blue lines, and bi-exciton DOSs are in red. Shown in (c) and (d) are the exciton-to-biexciton and bi-exciton-to-exciton rates R1→2 , R2→1 in CNT (6,2) and (6,5), respectively. Note that recombination rate magnitude—the dashed curves in (c) and (d—has been multiplied by 100. Our results indicate (see Fig. 4) that time evolution occurs on time scales that are much longer than the intrinsic times ~/E22 ∼ 3 × 10−16 s. This confirms the applicability of the BE approach to the dynamics of SWCNTs. Next, we augmented the system of equations for nα (t) with the MEG terms. Now as the excitation is cascading down the energy levels by emitting and absorbing phonons, it can, also, undergo an exciton → bi-exciton decay. Conversely, the bi-exciton state can recombine into a single high-energy exciton. For completeness, the exciton and bi-exciton spectra, as well as the exciton → bi-exciton rates from Refs. 24 and 25, are shown in Fig. 5. These results suggest that MEG strength in SWCNTs is likely to be determined by an intricate interplay between the Auger processes and phonon-mediated relaxation. For instance, just above the 2E g threshold there are energy ranges where bi-exciton density of states (DOS) is lower than the DOS of single excitons [Figs. 5(a) and 5(b)]. Counterintuitively enough, the faster phonon-mediated relaxation will carry the excitation through these energy ranges the smaller fraction of bi-excitons will be able to recombine, thus enhancing MEG. Also, we note that for efficient MEG it is crucial to have non-zero R1→2 just above the 2E g threshold. Using the QE procedure outlined in Sec. II B, we computed QE for the CNTs (6,2) and (6,5) as a function of the excitation energy. Our results are shown in Fig. 6. We predict efficient solar range MEG in both of these systems which starts at the threshold and reaches ∼1.6 at about 3E g . As already mentioned above, MEG in CNT (6,5) has been studied experimentally in Ref. 13. QE was measured for two opt excitation energies: for E = 2.5Eg , QE = 1.1 was reported, FIG. 6. The QEs for the CNT (6,2) and (6,5) vs. E/E g , where E g = 0.98 eV for (6,2) and for (6,5) E g = 1.09 eV. Vertical dashed line indicates the 2EgBSE threshold. 154106-8 Kryjevski et al. J. Chem. Phys. 147, 154106 (2017) opt while our prediction is QE ' 1.2, and for E = 3Eg , QE = 1.3 vs. QE ' 1.6, which is our prediction. The ways to improve accuracy of our method are discussed in Sec. V. V. CONCLUSIONS AND OUTLOOK We have used the Kadanoff-Baym-Keldysh technique of MBPT to develop a comprehensive DFT-based description of time evolution of a photoexcited SWCNT. The approach is based on the Boltzmann transport equation for time evolution of a weakly non-equilibrium photoexcited state in the quasiclassical limit with collision integrals calculated from the DFTbased Keldysh MBPT. We have been working to the second order in the RPA-screened Coulomb interaction and including electron-hole bound state effects for which we had to solve BSE. This method has been used to study MEG in the chiral SWCNTs, using (6,2) and (6,5) as examples. In particular, we calculated predictions for the internal QE as a function of the excitation energy. Our calculations suggest that chiral SWCNTs may have efficient MEG within the solar spectrum range (see Fig. 6). In the pristine SWCNTs, the MEG rates vary strongly with the excitation energy. In contrast, using the Cl-decorated (6,2) SWCNT as an example, it has been found that surface functionalization significantly alters low-energy spectrum in a SWCNT.25 Also, in the doped case, the MEG rate is not only greater in magnitude but also is a much smoother function of the excitation energy. QE calculations for the doped SWCNTs and for different chiral SWCNTs are in progress. As described above, several simplifying approximations had to be utilized in order to be able to calculate properties of these SWCNTs. Previously, we have checked that our predictions for the absorption spectra were in a reasonable agreement with the experimental data with the error less than 13% for E11 and E22 peak energies for the (6,2), (6,5), and (10,5) nanotubes. As discussed in Sec. IV, in this work we compared our predictions for the phonon-mediated relaxation and for QE(E) to the available experimental results for CNT (6,5). The comparison indicated that our current method is valid for SWCNTs at the semi-quantitative level. However, accuracy can be improved in several ways. For instance, static interaction approximation Π(ω, k, p) = Π(0, k, p) is reasonably accurate when employed in the BSE. But in the impact ionization process, the typical energy exchange is of order of the gap and, so, screening should be treated as dynamical. This is likely to enhance screening [see Eq. (9) for ω ' Eg ] which could help alleviate the overbinding issue. Implementation of this is technically challenging and is left to future work. A straightforward improvement is to include GW single particle energy corrections, which then can be easily incorporated in the rate expressions. It is likely to blue-shift the rate curves by a fraction of eV without significant changes to the overall shape. Another natural but technically challenging step is to use full RPA interaction W(ω, k, p) rather than W(0, k, k). However, none of these corrections are likely to change the main results and conclusions of this work while drastically increasing computational cost. ACKNOWLEDGMENTS Authors acknowledge financial support from NSF Grant No. CHE-1413614. S.K. acknowledges partial support of the Alfred P. Sloan Research Fellowship No. BR2014-073 and NDSU Advance FORWARD program sponsored by NSF Nos. HRD-0811239 and EPS-0814442. The authors acknowledge the use of computational resources at the Center for Computationally Assisted Science and Technology (CCAST) at North Dakota State University and the National Energy Research Scientific Computing Center (NERSC) allocation Award No. 86678, supported by the Office of Science of the DOE under Contract No. DE-AC02-05CH11231. 1 W. Shockley and H. Queisser, J. Appl. Phys. 32, 510 (1961). 2 R. J. Ellingson, M. C. Beard, J. C. Johnson, P. R. Yu, O. I. Micic, A. J. Nozik, A. Shabaev, and A. L. Efros, Nano Lett. 5, 865 (2005). J. Nozik, Phys. E 14, 115 (2002). 4 W. D. A. M. de Boer, E. M. L. D. de Jong, D. Timmerman, T. Gregorkiewicz, H. Zhang, W. J. Buma, A. N. Poddubny, A. A. Prokofiev, and I. N. Yassievich, Phys. Rev. B 88, 155304 (2013). 5 J. Stewart, L. Padilha, W. Bae, W. Koh, J. Pietryga, and V. Klimov, J. Phys. Chem. Lett. 4, 2061 (2013). 6 J. Bude and K. Hess, J. Appl. Phys. 72, 3554 (1992). 7 H. K. Jung, K. Taniguchi, and C. Hamaguchi, J. Appl. Phys. 79, 2473 (1996). 8 D. Harrison, R. A. Abram, and S. Brand, J. Appl. Phys. 85, 8186 (1999). 9 A. Nozik, Annu. Rev. Phys. Chem. 52, 193 (2001). 10 J. McGuire, M. Sykora, J. Joo, J. Pietryga, and V. Klimov, Nano Lett. 10, 2049 (2010). 11 N. M. Gabor, Acc. Chem. Res. 46, 1348 (2013). 12 O. Semonin, J. Luther, S. Choi, H.-Y. Chen, J. Gao, A. J. Nozik, and M. C. Beard, Science 334, 1530 (2011). 13 S. Wang, M. Khafizov, X. Tu, M. Zheng, and T. Krauss, Nano Lett. 10, 2381 (2010). 14 M. L. Bohm, T. C. Jellicoe, M. Tabachnyk, N. J. L. K. Davis, F. WisniveskyRocca-Rivarola, C. Ducati, B. Ehrler, A. A. Bakulin, and N. C. Greenham, Nano Lett. 15, 7987 (2015). 15 M. L. Bohm, M. Tabachnyk, F. Wisnivesky-Rocca-Rivarola, T. C. Jellicoe, C. Ducati, B. Ehrler, and N. C. Greenham, Nat. Commun. 6, 8259 (2015). 16 S. Saeed, C. de Weerd, P. Stallinga, F. Spoor, A. Houtepen, L. Siebbeles, and T. Gregorkiewicz, Light: Sci. Appl. 4, e251 (2015). 17 M. T. Trinh, R. Limpens, W. de Boer, J. Schins, L. Siebbeles, and T. Gregorkiewicz, Nat. Photonics 6, 316 (2012). 18 N. Gabor, Z. Zhong, K. Bosnick, J. Park, and P. McEuen, Science 325, 1367 (2009). 19 V. Perebeinos and P. Avouris, Phys. Rev. B 74, 121410 (2006). 20 S. Konabe and S. Okada, Phys. Rev. Lett. 108, 227401 (2012). 21 K. Velizhanin and A. Piryatinski, Phys. Rev. Lett. 106, 207401 (2011). 22 K. A. Velizhanin and A. Piryatinski, Phys. Rev. B 86, 165319 (2012). 23 S. Kilina, D. Kilin, and S. Tretiak, Chem. Rev. 115, 5929 (2015). 24 A. Kryjevski, B. Gifford, S. Kilina, and D. Kilin, J. Chem. Phys. 145, 154112 (2016). 25 A. Kryjevski, D. Mihaylov, B. Gifford, and D. Kilin, J. Chem. Phys. 147, 034106 (2017). 26 I. Marri, M. Govoni, and S. Ossicini, J. Am. Chem. Soc. 136, 13257 (2014). 27 L. Kadanoff and G. Baym, Quantum Statistical Mechanics (W. A. Benjamin, Inc., New York, 1962). 28 L. V. Keldysh, Zh. Eksp. Teor. Fiz. 47, 1515 (1964) [Sov. Phys. JETP 20, 1018 (1965)]. 29 E. M. Lifshitz and L. P. Pitaevskii, Physical Kinetics, 1st ed. (Pergamon Press, New York, 1981). 30 A. L. Fetter and J. Walecka, Quantum Theory of Many-Particle Systems (McGraw-Hill, New York, 1971). 31 G. Mahan, Many-Particle Physics, 2nd ed. (Plenum, New York, N.Y., 1993). 32 A. Kryjevski and D. Kilin, Mol. Phys. 112, 430 (2014). 33 G. Onida, L. Reining, and A. Rubio, Rev. Mod. Phys. 74, 601 (2002). 34 S. Kümmel and L. Kronik, Rev. Mod. Phys. 80, 3 (2008). 35 M. Rohlfing and S. Louie, Phys. Rev. B 62, 4927 (2000). 36 G. Strinati, Phys. Rev. B 29, 5718 (1984). 37 V. Berestetskii, E. Lifshitz, and L. Pitaevskii, Quantum Electrodynamics (Pergamon Press, Oxford, UK, 1979). 3 A. 154106-9 38 S. Kryjevski et al. Beane, P. Bedaque, W. Haxton, D. Phillips, and M. Savage, in At the Frontier of Particle Physics, edited by M. Shifman (World Scientific, 2000), Vol. 1, p. 133. 39 C. Spataru, S. Ismail-Beigi, L. Benedict, and S. Louie, Phys. Rev. Lett. 92, 077402 (2004). 40 V. Perebeinos, J. Tersoff, and P. Avouris, Phys. Rev. Lett. 92, 257402 (2004). 41 C. Spataru, S. Ismail-Beigi, R. Capaz, and S. Louie, Phys. Rev. Lett. 95, 247402 (2005). 42 S. Öğüt, R. Burdick, Y. Saad, and J. Chelikowsky, Phys. Rev. Lett. 90, 127401 (2003). 43 L. Benedict, A. Puzder, A. Williamson, J. Grossman, G. Galli, J. Klepeis, J.-Y. Raty, and O. Pankratov, Phys. Rev. B 68, 085310 (2003). 44 H. Wilson, D. Lu, F. Gygi, and G. Galli, Phys. Rev. B 79, 245106 (2009). 45 O. Vydrov, J. Heyd, A. Krukau, and G. Scuseria, J. Chem. Phys. 125, 074106 (2006). 46 J. Heyd, G. Scuseria, and M. Ernzerhof, J. Chem. Phys. 124, 219906 (2006). 47 J. Muscat, A. Wander, and N. Harrison, Chem. Phys. Lett. 342, 397 (2001). 48 M. Govoni and G. Galli, J. Chem. Theory Comput. 11, 2680 (2015). 49 M. Jain, J. Chelikowsky, and S. Louie, Phys. Rev. Lett. 107, 216806 (2011). 50 M. Hybertsen and S. Louie, Phys. Rev. B 34, 5390 (1986). 51 J. Noffsinger, E. Kioupakis, C. Van de Walle, S. Louie, and M. Cohen, Phys. Rev. Lett. 108, 167402 (2012). 52 P. Han and G. Bester, Phys. Rev. B 91, 085305 (2015). J. Chem. Phys. 147, 154106 (2017) 53 A. Kryjevski, in Toward First-Principles Description of Carrier Relaxation in Nanoparticles in Photoinduced Processes at Surfaces and in Nanomaterials, ACS Symposium Series (ACS Publications, 2015), Vol. 1196, Chap. 10, pp. 201–213. 54 D. T. Devreese and P. van Camp, Electronic Structure, Dynamics, and Quantum Structural Properties of Condensed Matter (Springer, New York, 1985). 55 P. Han and G. Bester, Phys. Rev. B 85, 235422 (2012). 56 X. Gonze, P. Boulanger, and M. Cote, Ann. Phys. 523, 168 (2011). 57 A. A. Abrikosov, L. Gorkov, and I. E. Dzyaloshinski, Methods of Quantum Field Theory in Statistical Physics (Prentice-Hall, Englewood Cliffs, NJ, 1963). 58 P. E. Blöchl, Phys. Rev. B 50, 17953 (1994). 59 G. Kresse and D. Joubert, Phys. Rev. B 59, 1758 (1999). 60 M. W. Graham, T. R. Calhoun, A. A. Green, M. C. Hersam, and G. R. Fleming, Nano Lett. 12, 813 (2012). 61 C. Manzoni, A. Gambetta, E. Menna, M. Meneghetti, G. Lanzani, and G. Cerullo, Phys. Rev. Lett. 94, 207401 (2005). 62 A. Gambetta, C. Manzoni, E. Menna, M. Meneghetti, G. Cerullo, G. Lanzani, S. Tretiak, A. Piryatinski, A. Saxena, R. L. Martin et al., Nat. Phys. 2, 515 (2006). 63 S. Kilina, S. Tretiak, S. Doorn, Z. Luo, F. Papadimitrakopoulos, A. Piryatinski, A. Saxena, and A. Bishop, Proc. Natl. Acad. Sci. U. S. A. 105, 6797 (2008).

1/--страниц